Active Standard ASTM D2653 | Developed by Subcommittee: D13.58
Book of Standards Volume: 07.01
Historical (view previous versions of standard)
Significance and Use
This test method is considered satisfactory for acceptance testing of commercial shipments since current estimates of between-laboratory precision are acceptable and the method is used extensively in the trade for acceptance testing.
If there are differences of practical significance between reported test results for two laboratories (or more), comparative tests should be performed to determine if there is a statistical bias between them, using competent statistical assistance. As a minimum, use samples for such comparative tests that are as homogeneous as possible, drawn from the same lot of material as the samples that resulted in disparate results during initial testing, and randomly assigned in equal numbers to each laboratory. The test results from the laboratories involved should be compared using a statistical test for unpaired data, at a probability level chosen prior to the testing series. If bias is found, either its cause must be found and corrected, or future test results for that material must be adjusted in consideration of the known bias.
The force at first filament break of elastomeric yarns may depend on its construction and manufacturing process and provides an indication of the breaking strength of fabrics made from the yarn.
Elongation is an indication of the ability of a fiber to absorb energy. The elongation of yarn or fabric must be great enough to withstand strains experienced in processing and end use, and to absorb the energies of applied forces repeatedly.
Fabric manufacturers use force and elongation information of elastomeric yarns in determining machine set-up conditions.
Other parameters such as elongation at specified force (EASF), force (or tenacity) at specified elongation (FASE, TASE), work and toughness may be calculated from force-elongation curves. EASF and FASE information is needed for tests involving cycling of yarn in determination of elastic properties.
This test method was developed using elastomeric yarns in the “as-produced” condition, but may be used for treated elastomeric yarns provided the treatment is specified. The method does not cover the removal of finish for determination of tensile properties of “finish-free” elastomeric yarns.
1.1 This test method covers the determination of the tensile properties of “as produced” elastomeric yarns made from natural rubber, spandex or other elastomers, using a constant-rate-of-extension (CRE) type tensile testing machine. The properties included in this test method are: (1) force at first filament break, (2) tenacity at first filament break, (3) elongation at first filament break, (4) work to break at first filament break, and (5) toughness at first filament break.
1.2 This test method does not apply to covered, wrapped, or core-spun yarns or yarns spun from elastomeric staple.
1.3 This test method is applicable to elastomeric yarns in the range from 40 to 3200 dtex (36 to 2900 denier).
1.4 The values stated in either SI units or U.S. Customary units are to be regarded separately as standard. Within the text, the U.S. Customary units are given in parentheses. The values stated in each system are not exact equivalents; therefore, each system shall be used independently of the other.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D76 Specification for Tensile Testing Machines for Textiles
D123 Terminology Relating to Textiles
D1776 Practice for Conditioning and Testing Textiles
D2258 Practice for Sampling Yarn for Testing
D2591 Test Method for Linear Density of Elastomeric Yarns (Short Length Specimens)
D4848 Terminology Related to Force, Deformation and Related Properties of Textiles
D4849 Terminology Related to Yarns and Fibers
D6717 Test Method for Linear Density of Elastomeric Yarns (Skein Specimens)
ICS Number Code 59.080.20 (Yarns)